Effects of Plasmonic Metal Core -Dielectric Shell ... › publication › fulltext › Effects-of... › publication › fulltext › Effects-of...by P Yu · Cited by 78 — This work provides a concept to achieve enhanced forward scattering with weakened backward ... M
Received: 6 June 2017 Accepted: 6 July 2017 Published: xx xx xxxx
Effects of Plasmonic Metal Core -Dielectric Shell Nanoparticles on the Broadband Light Absorption Enhancement in Thin Film Solar Cells Peng Yu 1, Yisen Yao1, Jiang Wu2, Xiaobin Niu3, Andrey L. Rogach 4 & Zhiming Wang1 To guide the design of plasmonic solar cells, theoretical investigation of core (metal)-shell (dielectric) nanoparticles for light absorption enhancement in thin film Si solar cells is performed. In contrast to the reported simulations and experimental results that rear-located surface plasmon on bare metallic nanoparticles is preferred, the core-shell nanoparticles demonstrate better performance when surface plasmon is located in front of a solar cell. This has been attributed to the enhanced forward scattering with vanishing backward scattering preserved over a wide spectral range in core-shell nanoparticles. This work provides a concept to achieve enhanced forward scattering with weakened backward scattering in plasmonic thin film solar cells. Solar energy is an ideal candidate for addressing the energy crisis and reducing carbon emission. Efficient light management schemes are crucially important to maintain high efficiency of photovoltaic (PV) devices such as thin film solar cells, quantum dot solar cells, nanostructured solar cells, and plasmonic solar cells. Thin film solar cells offer the advantage of reduced material costs, but they incur transmission losses and reduce cell performance as absorber layers become thinner1. Surface texturing is the main method for commercial solar cells to boost efficiencies, but it is not compatible with thin film solar cells. Quantum dot (QD) solar cells have the potential to boost the maximum attainable thermodynamic conversion efficiency of solar photon conversion up to ~66%2. However, they are still suffering from poor optical and electrical properties of QDs grown by mainstream Stranski-Krastanov method, because the strain accumulation from the stacking multiple QDs introduces lattice defects which are detrimental to device performance3. The nanostructured solar cells such as those based on the close-packed nanowires4–6 are beneficial for the absorption at longer wavelengths, but the device performance is vulnerable to the surface recombination due to the large surface-area-to-volume ratio7. The plasmonic light-trapping scheme attracted a lot of attention to aid photocurrent enhancement in solar-cells8–13. Incorporating plasmonic enhancers into thin film solar cells helps to achieve higher power conversion efficiency (PCE) while lessening physical thickness of the materials significantly. This approach makes use of collective oscillation of excited free electrons in noble metal nanoparticles, which are influenced by particle shape, size and dielectric properties of the surrounding medium, and surface coverag14. Catchpole et al. have shown that metal nanoparticles with cylindrical and hemispherical geometry lead to a much higher path length enhancements than their spherical counterpart15. Another of their works demonstrated that resonant surface plasmon polariton modes, supported by disk-shaped metal nanoparticles on high-index substrates, is very sensitive to the area in contact with the substrate and insensitive to particle height16. J. Wu et al. coupled Au and Ag nanoparticles on InAs/GaAs QD solar cell surfaces and presented an overall PCE enhancement from 8.0% to 9.5% and 8.9% 1
Institute of Fundamental and Frontier Science, University of Electronic Science and Technology of China, Chengdu, 610054, P. R. China. 2Department of Electronic and Electrical Engineering, University College London, Torrington Place, London, WC1E 7JE, United Kingdom. 3State Key Laboratory of Electronic Thin Film and Integrated Devices, University of Electronic Science and Technology of China, Chengdu, 610054, P.R. China. 4Department of Physics and Materials Science and Centre for Functional Photonics (CFP), City University of Hong Kong, Hong Kong SAR, P. R. China. Correspondence and requests for materials should be addressed to J.W. (email: [email protected]
) or Z.W. (email: [email protected]
) SCIEnTIFIC Reports | 7: 7696 | DOI:10.1038/s41598-017-08077-9
Figure 1. Four possible photophysical processes of core-shell nanoparticle in contact with Si solar cells. (a) Near-field coupling. (b) Far-field scattering. (c) Hot electron transfer. (d) Plasmon resonant energy transfer.
respectively17. Size-controlled Ag nanoparticles with high aspect-ratio resulted in an 8% increase in the short circuit density of GaAs solar cells18. Self-assembled Ag nanoparticle-based plasmonic back reflector in a-Si:H cell achieved a short circuit current as high as 15.1 mA/cm2 19. Metal nanostructured plasmonic sources, such as nanospheres17–19, nanostars20, nanocages21, nanodisks22, nanocavity23, nanovoids24, nucleated nanoparticles25, have been all demonstrated for optical absorption enhancement. Plasmonics also opens an avenue for achieving panchromatic solar cell conversion designs, es